Crystals 2015 5, 355-375; doi:10.3390/cryst5030355 OPEN ... · PDF file Crystals 2015, 5,...
Embed Size (px)
Transcript of Crystals 2015 5, 355-375; doi:10.3390/cryst5030355 OPEN ... · PDF file Crystals 2015, 5,...
Crystals 2015, 5, 355-375; doi:10.3390/cryst5030355
crystals ISSN 2073-4352
Dendrite Growth Kinetics in Undercooled Melts of Intermetallic Compounds
Dieter M. Herlach
Institut für Materialphysik im Weltraum, Deutsches Zentrum für Luft- und Raumfahrt, DLR, Köln 51147, Germany; E-Mail: [email protected]; Tel.: +49-2203-6012332; Fax: +49-2203-61768
Academic Editor: Duc Nguyen-Manh
Received: 2 June 2015 / Accepted: 27 August 2015 / Published: 7 September 2015
Abstract: Solidification needs an undercooling to drive the solidification front. If large undercoolings are achieved, metastable solid materials are solidified from the undercooled melt. Containerless processing provides the conditions to achieve large undercoolings since heterogeneous nucleation on container walls is completely avoided. In the present contribution both electromagnetic and electrostatic levitation are applied. The velocity of rapidly advancing dendrites is measured as a function of undercooling by a High-Speed-Camera. The dendrite growth dynamics is investigated in undercooled melts of intermetallic compounds. The Al50Ni50 alloy is studied with respect to disorder trapping that leads to a disordered superlattice structure if the melt is undercooled beyond a critical undercooling. Disorder trapping is evidenced by in situ energy dispersive diffraction using synchrotron radiation of high intensity to record full diffraction pattern on levitated samples within a short time interval. Experiments on Ni2B using different processing techniques of varying the level of convection reveal convection-induced faceting of rapidly growing dendrites. Eventually, the growth velocity is measured in an undercooled melt of glass forming Cu50Zr50 alloy. A maximum in the growth velocity–undercooling relation is proved. This is understood by the fact that the temperature dependent diffusion coefficient counteracts the thermodynamic driving force for rapid growth if the temperature of the undercooled melt is approaching the temperature regime above the glass transition temperature. The analysis of this result allows for determining the activation energy of atomic attachment kinetics at the solid–liquid interface that is comparable to the activation energy of atomic diffusion as determined by independent measurements of the atomic diffusion in undercooled Cu50Zr50 alloy melt.
Crystals 2015, 5 356
Keywords: containerless processing; undercooling of melts; intermetallics; metastable solids
Metallic materials are prepared from the liquid state as their parent phase. To date, efforts are directed towards virtual material design with computer-assisted modeling. Computational materials science from the liquid state requires detailed knowledge of the physical mechanisms involved in the solidification process. In particular, these are crystal nucleation and crystal growth. Both of these processes are driven by an undercooling of the liquid below its equilibrium melting temperature to develop conditions where a driving force for the formation of supercritical nuclei and the advancement of a solidification front is created. This gives access to non-equilibrium solidification pathways, which can form metastable solids, which may differ in their physical and chemical properties from their stable counterparts. Detailed modeling of solidification, far away from thermodynamic equilibrium, requires that the solidification process has to be investigated in every detail.
In order to achieve the state of an undercooled melt, it is advantageous to remove heterogeneous nucleation sites, which otherwise limit the undercoolability. The most efficient way to realize such conditions is containerless processing of melts . In such, the most dominant heterogeneous nucleation process, involving interaction with container walls, is completely avoided. Electromagnetic  and electrostatic levitation techniques [3,4] have been developed for containerless undercooling and solidification of molten metals and alloys. A freely suspended drop gives the extra benefit to directly observe the solidification process by combining the levitation technique with proper diagnostic means [5,6]. Short range ordering in undercooled metallic melts as precursor of crystal nucleation has been investigated by using neutron diffraction  and synchrotron radiation  on containerless undercooled melts . In particular, containerless processing under ultra high vacuum condition is favorable to achieve large undercoolings from which the interfacial energy between crystal nucleus and undercooled melt may be inferred. Rapid growth of dendrites is observed on levitation undercooled melts by using high speed video camera techniques characterized by high spatial and temporal resolution . In the case of containerless processing, heat is transferred by heat radiation and additionally by heat conduction in an environmental gas if the sample is processed in an inert noble gas atmosphere (e.g., in electromagnetic levitation). If the sample is largely undercooled prior to solidification, the initial crystallization process is very rapid. As a consequence the undercooled melt serves as a heat sink. This leads to a temperature rise during the initial crystallization of the sample known as recalescence.
By analyzing measured temperature–time profiles and measurements of the dendrite growth velocity as a function of undercooling disorder trapping is investigated on intermetallic compounds. Dendrite growth is controlled by heat and mass redistribution. Thus, any transport process stimulated externally by natural convection and/or forced convection due to stirring effects of alternating electromagnetic fields and/or natural convection may cause serious influence on the solidification process. To understand this effect and to develop a quantitative description of crystallization in the presence of forced convection, comparative experiments on Earth and in reduced gravity are of great help. Under the special conditions of reduced gravity, for instance in Space, the forces needed to compensate disturbing
Crystals 2015, 5 357 accelerations are about three orders of magnitude smaller than the forces needed to compensate the gravitational force for levitation experiments on Earth. In a cooperative effort by the European Space Agency (ESA) and the German Aerospace Center—Space Management (DLR) a facility for Electro-Magnetic Levitation (EML) has been developed and was accommodated in the European module Columbus of the International Space Station (ISS) in August 2014. International research teams prepared experiments using the EML multiuser facility for investigations on undercooled metallic melts in Space .
The present article aims to give an overview of the present state of investigations of dendrite growth in undercooled melts of intermetallic compounds.
2. Experimental Details
Samples were prepared from alloy constituents all of purity of 4N5. The weight components are pre-melted in an arc furnace under high purity argon gas (6N). The samples were placed and processed in the ultra-high-vacuum chambers of electromagnetic  and/or electrostatic levitator . The temperature is measured by pyrometers with an absolute accuracy of ±5 K. Samples in diameter of 7 mm are processed by electromagnetic levitation. The application of electromagnetic levitation is limited since levitation force and inductive heating is coupled. In order to cool the liquid sample forced convection by helium gas is used. In the electrostatic levitator samples in diameter of 2–3 mm are processed under ultrahigh vacuum conditions (≈10−8
mbar). Levitation and heating is decoupled in
contrast to the electromagnetic levitator. A high-speed video camera (Photron VKT, Video Kommunikation GmbH, Pfullingen, Germany) was applied (frame rate up to 50,000 pictures per second) to record the rapid advancement of the intersection line of the solidification front and the sample surface. A method has been developed to infer the velocity of the dendrites propagating within the bulk of the melt by projection of the interface of the solidification front and the sample surface into the interior of the drop shaped sample . In this way, rapid dendrite growth velocity is measured as a function of undercooling. The measurements of dendrite growth in undercooled melts of Al50Ni50 and Ni2B alloys in reduced gravity were conducted using the TEMPUS facility for electromagnetic levitation in space  during parabolic flight campaigns.
3. Results and Discussions
3.1. Dendrite Growth Theory
Crystal growth in undercooled melts leads to heating up the solid–liquid interface due to the release of the heat of crystallization. As a consequence, a negative temperature gradient will be established in front of the interface since the undercooled melt acts as a heat sink. This will destabilize the initially planar interface. Due to limited solubility of the solute in the solid phase of alloys, compared to the liquid phase, solute will pile up in front of the interface. The resulting concentration gradient will reinforce, in addition to the negative temperature gradient, the instability of the solidification front. Eventually, the morphological destabilization of an initially planar interface will lead to dendrite growth . Dendrites consist of the main stem and side-branches, which grow into the melt.
Crystals 2015, 5 358
An extended model of sharp interface theory is applied to describe the gr